# Modeling of Random Quasi-Phase-Matching in Birefringent

date post

16-Feb-2022Category

## Documents

view

0download

0

Embed Size (px)

### Transcript of Modeling of Random Quasi-Phase-Matching in Birefringent

Jolanda S. Muller, Andrea Morandi, Rachel Grange, and Romolo Savo∗

Optical Nanomaterial Group, Institute for Quantum Electronics, Department of Physics, ETH Zurich, Zurich, Switzerland

(Dated: November 23, 2020)

We provide a vectorial model to simulate second-harmonic generation (SHG) in birefringent,

transparent media with an arbitrary configuration of nonlinear (χ(2)) crystalline grains. We apply this model on disordered assemblies of LiNbO3 and BaTiO3 grains to identify the influence of the birefringence on the random quasi-phase-matching process. We show that in monodispersed assem- blies, the birefringence relaxes the grain size dependence of the SHG efficiency. In polydispersed assemblies with sufficiently large grains, we find that the birefringence introduces an SHG efficiency enhancement of up to 54% compared to isotropic reference crystals, which is grain size independent. This enhancement increases linearly with the grain size, if the birefringent grains can be phase matched. These two different scaling behaviours are used in Kurtz and Perry’s powder-technique to identify the phase-matchability of a material. We show on the example of LiNbO3 and ADP that this technique cannot be applied when the grains get smaller than the coherence length, because the SHG scaling with the grain size becomes material specific.

Optical frequency conversion through phase match- ing in birefringent nonlinear (χ(2)) crystals has enabled a variety of applications in laser technology [1, 2] and plays a key role in quantum source schemes [3]. The birefringence provides an orientation- and polarization- dependent refractive index, which is used to compen- sate for the phase lag accumulated by the mixing waves. This avoids the destructive interference of the generated waves, which starts to occur at lengths larger than the co- herence length in any not phase-matched configuration. Random quasi-phase-matching (RQPM) is an alternative approach for removing destructive interference in optical frequency conversion [4, 5]. It relies on the disordered dis- tribution of the χ(2)-domains of certain media, such as polycrystalline materials [5–7], scattering powders [8–11] and bottom-up assembled photonic structures [12, 13]. Under a pump excitation the domains, or grains, gener- ate nonlinear waves with random phases and amplitudes. This leads to the cancellation of the interference terms and to the linear accumulation of the generated power with the number of domains. While RQPM is gener- ally less efficient than phase matching, it provides numer- ous advantages, such as an ultra-broad acceptance band- width (tunability of the pump over hundreds of nanome- ters), the use of low-cost materials, and relaxed con- straints on the polarization and the angle of incidence of the pump. These features make RQPM attractive for a variety of applications, such as optical-parametric- oscillators [14], ultrafast mid-infrared lasers [15], and ul- trafast autocorrelators [16]. The interest on RQPM has been largely focused on isotropic (i.e. non-birefringent) crystals such as ZnSe, both experimentally and theoret- ically [5, 17, 18]—one reason for this is that RQPM en- ables taking advantage of the large nonlinearity of these isotropic crystals, even if they are non-phase-matchable. First modeling of RQPM relied on the scalar approxima-

∗ [email protected]

tion of both the optical field and the χ(2)-susceptibiliy of the grains [17, 19]. Very recently, more comprehensive vectorial models have been developed to study the non- linear speckle statistics [18] and the supercontinuum gen- eration from isotropic disordered polycrystals [20]. SHG in birefringent disordered materials has only been mod- eled by averaging over the single grain generation, with- out considering the effects of the propagation through the birefringent medium on the polarization states [21, 22]. Up to now, no comprehensive model that explicitly ac- counts for the birefringence in RQPM has been presented.

Here, we introduce a vectorial model that considers the full three dimensional rotation (i.e. full χ(2)-tensor) as well as the birefringence of each grain. The generation and propagation of the waves is calculated from grain-to- grain, considering the phases of the ordinary and extraor- dinary beam components separately. This is done within the approximation of no scattering at the grain-to-grain boundaries. We explore the effects of the birefringence on RQPM by calculating the second-harmonic genera- tion (SHG) in disordered assemblies of lithium niobate (LiNbO3) and barium titanate (BaTiO3). We find that in general the birefringence is beneficial for RQPM. In monodispersed assemblies, the birefringence relaxes the grain size dependence of the SHG efficiency. In poly- dispersed assemblies, it introduces an efficiency enhance- ment of up to 54% compared to an isotropic reference material. Thanks to the birefringence, our model can simulate grains in a phase-matchable regime, in which the SHG enhancement increases linearly with the grain size. This allows us to draw a comparison to the powder- characterization technique of Kurtz and Perry [8, 22], which is widely applied to identify the phase-matchability of a crystalline material. Contrary to the established be- haviour at large grain sizes, we find that the SHG scal- ing with the grain size cannot unequivocally identify the phase-matchability of a crystal when the grain size is smaller than the coherence length.

ar X

iv :2

01 1.

10 42

9v 1

I. MODEL

The presented model considers a disordered three dimensional cuboid structure, consisting of quadratic (χ(2) 6= 0), birefringent, crystalline grains, as depicted in Fig. 1a. Similarly to other models [17, 18], the three di- mensional problem is reduced to a one dimensional prob- lem by breaking down the cuboid into multiple paral- lel one dimensional sticks. The SHG of each individual stick is calculated separately. Fig. 1b shows one disor- der configuration of such a stick, in which the grains have random sizes and orientations. The size Xn is ran- domly chosen from a Gaussian distribution with an av- erage grain size X and a polydispersity σ. The random orientation is defined through the rotation between the lab frame (a,b,c) and the crystal frame of each grain (x,y,z), with the Euler angles (, ϑ, γ)n, as shown in Fig. 1e. For this, the lab frame axes are defined as the c-axis parallel to the propagation direction k and the two orthogonal directions a and b, while the z axis is the optic axis of the crystal. For a uniform distri- bution of crystal orientations, we choose the rotation around z as ∈ [0, 2π], the angle between k and z as ϑ = arccos(u) with u ∈ [−1, 1] [18], and the rotation around k as γ ∈ [0, 2π]. The refractive indices of the ordinary (o) and extraordinary (e) axes are given by no

and ne(ϑ) = (

)−1/2 , with ne

the extraordinary refractive index at ϑ = π/2 [1]. A visu- alization of the calculation process in one single grain is shown in Fig. 1d. The incoming beam (pump) is defined as the plane wave (red)

E(ω) = (eaeiφa cosβ + ebeiφb sinβ)Eωe i(kc−ωt)

with amplitude Eω, frequency ω, wavevector k, the start- ing phases φa and φb, and a polarisation angle β in the lab frame. The vectors ea and eb are the unit vectors along the a and b axes. At the beginning of the grain, the elec- tric fields in the lab frame Elab, are transformed into the reference frame of the respective crystal Ecry = R ·Elab

(Fig. 1e), where R = Z1()X2(ϑ)Z3(γ) is the Euler- transformation matrix for a rotation around the original z-axis (Z1 = z) by , the new x-axis (X2 = o) by ϑ and final z-axis (Z3 = k) by γ (see Supplementaries II). In the crystal frame (Fig. 1d), the beams are decomposed into their components along the o and e axes and each polarisation combination of the pump (oo, eo, oe, ee) gen- erates a second-harmonic field Eugen(2ω,Xn) (blue) along

u ∈ {o, e}, which is given at the end of the nth single grain according to:

Eugen(2ω,Xn) = ∑

v,w

i(2ω)2

u 3Xn

(1) With the phase mismatch ku,vw = kv(ω) + kw(ω) − ku(2ω), the wave vector ku3 of the second-harmonic along u, and Pu,vw = eu,P vw the second-harmonic po- larization along v, w ∈ {o, e} projected onto the o/e-

FIG. 1. (a) Sketch of a three dimensional disordered assembly of second-order nonlinear grains, consisting of multiple par- allel one dimensional sticks. (b) Each stick contains grains of varying size Xn and orientation (, ϑ, γ)n, represented by the variation in colour. (c) Phasor (an) representation of the interference between the second-harmonic waves gener- ated by the grains within the stick. Each stick corresponds to a single random walk in the SHG complex plane, in which the step length is the amplitude of the second-harmonic field. (d) Schematics of the process to propagate, generate and in- terfere the beams. The input (left) is transformed into the crystal frame, propagated, summed with the generated SHG, and transformed back into the lab frame. (e) Depiction of the angles between the crystal frame (x,y,z) and the lab frame (a,b,c) with the transformation matrix R. β is the polarisa- tion angle of the input beam in case of a linearly polarized beam (φa = φb). The ordinary/extraordinary axes are indi- cated with o and e.

axis (eu unit vector along u ∈ {o, e}), where P vwi = 2ε0 ∑ jk dijkE

v jE

w k . The second-order nonlinear tensor

dijk is used in its contracted matrix form to calculate P vwi (see Supplementaries II). The pump E(ω, 0), as well as the total second-harmonic from all previous crystals Epre(2ω, 0) are propagated through the grain. For both beams, the components along the o and e axis are prop- agated separately: Eu(ω,Xn) = Eu(ω, 0)eik

u(ω)Xn . At the end of the grain, the second-harmonic from the pre-

3

vious grains is summed with the second-harmonic gener- ated in the current grain Eutot(2ω,Xn) = Eupre(2ω,Xn) + Eugen(2ω,Xn) (* in Fig. 1d). The amplitude, polarisation and phase of the fields is explicitly considered in every step. This way, the model can account for interference ef- fects. The fields of the propagated pump Eu(ω,Xn) and the total second-harmonic field Eutot(2ω,Xn) are trans- formed back into the lab frame, forming the output of the nth grain. To simulate the propagation of the light through the stick, we implemented a folding algo- rithm, which iteratively processes the sequence of grains. In each step, it takes the data of the current element (grain n) of the sequence and the result of the previous step (grain n−1) as input. The information is processed to generate the output of the nth grain which then forms the input of the (n+ 1)th grain. The SHG intensities of each stick Istick = cε0(|Eatot|2 + |Ebtot|2)/2 are averaged to yield the intensity of the cuboid. The model assumes an undepleted pump, no absorption within the grains, no reflections at the grain-to-grain interfaces, and the prop- agation only in the forward direction (no walk-off angle).

As an initial test of the algorithm, we computed the SHG from structures characterised by mono- and poly- dispersed grain sizes without randomisation of the grain orientation. The system behaves identical to a single crystal, periodically showing a totally constructive and destructive SHG along the length of the system. As ex- pected, there is no dependence on the size distribution of the grains (see Supplementaries III). When introduc- ing disorder in grain orientation and grain size, the SHG intensity of the single stick depends strongly on the spe- cific disorder configuration. In this case, the SHG in- terference along the stick corresponds to the trajectory of a single random walk in the complex plane, as de- picted in Fig. 1c. As such, the SHG intensity of a single stick cannot be correlated with the number of grains N . Only upon averaging the intensities of multiple sticks (i.e. along the transverse dimensions of the cuboid), the total SHG intensity grows linearly with N , providing evidence of RQPM [17]. To quantitatively study the influence of birefringence, we introduce the isotropic analogue of a birefringent material, defined as the material that has the same χ(2)-tensor as the original material, but with ne = no. Hence, the coherence length of the isotropic analogue Liso

c is not angle dependent. This stands in contrast to the coherence length in a birefringent mate- rial Lbir

c (, ϑ, γ)n, which depends on the angle, as well as the combination of beam polarizations. Thus, a random distribution of the grain orientations does not affect the coherence length of isotropic grains, while it randomises the coherence length of birefringent grains.

II. RESULTS

Monodispersed Assemblies.— One noteworthy result of this study, which is not exclusively related to birefrin- gence, is that even monodispersed structures (without

FIG. 2. Scaling of the SHG intensities with the number of grains N in birefringent LiNbO3 and in its isotropic analogue at a pump wavelength of 930 nm. SHG intensities are aver- aged over 1000 sticks, leading to a linear growth. Its slope represents the SHG efficiency for a certain grain size, and the shaded area shows the possible efficiencies in monodispersed assemblies. The insets explicitly show the SHG intensity in monodispersed assemblies only as a function of the grain size X for N = 100. In polydispersed assemblies (σ = 30%) with large grains (X > 3 Liso

c in the isotropic and X > 8 Liso c

in the birefringent material) the efficiency has a stable value corresponding to the dotted line. (a) The isotropic analogue has zero-efficiency minima when X is an even multiple of Liso

c , and efficiency maxima when X is an odd multiple of Liso

c . (b) The birefringent assembly has its minimum at X = 9.25 Liso

c

and its maximum at X = 3.47 Liso c .

size randomisation) sustain RQPM, as long as the grains are randomly oriented. This is shown in Fig. 2a-b for LiNbO3. The SHG efficiency per grain is measured by the slope of the linear growth, which depends on the grain size X. Its variation is represented by the shaded area and can be seen in the insets of Fig. 2a-b, which report the SHG intensity as a function of the grain size. The isotropic analogue, Fig. 2a, shows a maximal efficiency when X is an odd multiple of Liso

c and a minimal (zero) efficiency when X is an even multiple of Liso

c . The latter case corresponds to the totally destructive SHG inter- ference within the single grains. This is consistent with the results of Vidal. et al. [17] at low polydispersity. The effect of the birefringence is shown in Fig. 2b. The maximal as well as the minimal efficiency is increased compared to the isotropic analogue. In particular, the lower bound of the cone has a non-zero slope and the SHG never vanishes. Indeed, each birefringent grain has an orientation-dependent coherence length Lbir

c (, ϑ, γ)n, prompting that there is no specific grain size at which to- tal destructive interference occurs for all grains. BaTiO3

4

shows the same effect, but with a narrower cone of possi- ble efficiencies (see Supplementaries IV). The considered case of monodispersed assemblies highlights that polydis- persity is neither a sufficient nor a necessary condition to achieve RQPM. This stands in contrast to the random orientation of grains, which plays a key role in reaching the RQPM regime.

Polydispersed Assemblies.— In Fig. 3a the SHG in- tensity of LiNbO3 assemblies (red) and of their isotropic analogue (blue) is shown for an increasing average grain size 0 ≤ X ≤ 20 Liso

c , a polydispersity σ = 30%, and a fixed number of grains N = 100. Both curves follow the expected trend for RQPM [17]. In the small grain regime (X > Liso

c ) the SHG intensity grows with the grain size without an appreciable difference between the bire- fringent and the isotropic case. Maximal intensities are reached when X = Liso

c , for the isotropic analogue and for slightly larger grains in birefringent LiNbO3. After an initial peak, the SHG gets independent of the average grain size, at ≈ 3 Liso

c for the isotropic analogue and at ≈ 8 Liso

c for the birefringent LiNbO3. In this stabilised large-grain regime, the SHG intensity of the birefringent LiNbO3 is significantly larger than the stable value of the isotropic analogue. Specifically, we observe a peak enhancement of 54 ± 2% at 3 Liso

c . The effect is weaker in BaTiO3, where the birefringence leads to an SHG en- hancement of 9.25± 0.8% (see Supplementaries IV). The enhancement can also be seen on the slope of the of dot- ted lines in Fig. 2a-b, which report the linear scaling of the SHG intensity for assemblies with polydispersed grains at large grain sizes.

The origin of this overall enhancement lies in the dis- tribution of the SHG intensities generated by the indi- vidual grains Igen = cε0(|Eogen|2 + |Eegen|2)/2 within the cuboid, which are shown in Fig. 3b for both the bire- fringent (red) and the isotropic (blue) LiNbO3. These two SHG intensity distributions have been obtained by extracting Igen of the individual grains from the com- plete simulation depicted in Fig. 1d, thus considering the specific polarization state of the pump (phase retarda- tion between the o and e components) that the propaga- tion through the previous birefringent grains introduced. The birefringence significantly widens the range of pos- sible SHG intensities in the individual grains, due to the increased coherence lengths Lbir

c (, ϑ, γ)n > Liso c for cer-

tain grain orientations. Consequently, the average SHG intensity of the individual grains of birefringent LiNbO3

is 54.1± 0.3% higher than the isotropic analogue. Simi- larly for BaTiO3, the enhancement is 9.24± 0.1%, whose single-grain SHG intensity distribution is shown in the Supplementaries IV. The enhancements of Igen are con- sistent with the enhancement of the assembly calculated by considering the vectorial propagation of all compo- nents. We highlight that the birefringence is only bene- ficial in grains larger than the isotropic coherence length Xn > Liso

c . In smaller grains, the grain size Xn, rather than the coherence length, is the length scale limiting their SHG intensity (see Supplementaries V). To under-

FIG. 3. (a) Scaling of the SHG intensity with the average grain size for disordered assemblies of isotropic LiNbO3, bire- fringent LiNbO3, and birefringent LiNbO3 in the single grain (SG) approximation (single grain average ×N). The assem- blies have a grain size polydispersity σ = 30%, a fixed number of grains per stick N = 100, an averaging over 1000 sticks, and are simulated at a pump wavelength of 930 nm. At this wave- length, phase matching in LiNbO3 is not possible. (b) Proba- bility distributions of the SHG intensities generated by the in- dividual grains within the assembly (X = 3 Liso

c and σ = 30%) for isotropic LiNbO3, birefringent LiNbO3, and birefringent LiNbO3 in the single grain (SG) approximation (N = 1, lin- early polarized input beam). Probabilities are calculated as the relative frequency of appearance of an SHG intensity value over 107 grains. The SHG binning is 0.002. The SHG intensi- ties are multiplied by 100 to be directly comparable with the intensities of the 100-grain-assemblies in (a).

line the importance of modeling the phase propagation between the grains, we calculated the SHG scaling also in the single grain (SG) approximation, i.e. by consid- ering randomly oriented grains that are independently illuminated with a linearly polarized pump. Their aver- age SHG is then multiplied by N to get the SHG effi- ciency of the assembly ISG

tot = N × ISG gen. As shown in

Fig. 3a (grey line), the SG approximation overestimates the SHG enhancement in the birefringent assembly of LiNbO3 almost by a factor 2. This is because the SG approximation ignores the retardation…

Optical Nanomaterial Group, Institute for Quantum Electronics, Department of Physics, ETH Zurich, Zurich, Switzerland

(Dated: November 23, 2020)

We provide a vectorial model to simulate second-harmonic generation (SHG) in birefringent,

transparent media with an arbitrary configuration of nonlinear (χ(2)) crystalline grains. We apply this model on disordered assemblies of LiNbO3 and BaTiO3 grains to identify the influence of the birefringence on the random quasi-phase-matching process. We show that in monodispersed assem- blies, the birefringence relaxes the grain size dependence of the SHG efficiency. In polydispersed assemblies with sufficiently large grains, we find that the birefringence introduces an SHG efficiency enhancement of up to 54% compared to isotropic reference crystals, which is grain size independent. This enhancement increases linearly with the grain size, if the birefringent grains can be phase matched. These two different scaling behaviours are used in Kurtz and Perry’s powder-technique to identify the phase-matchability of a material. We show on the example of LiNbO3 and ADP that this technique cannot be applied when the grains get smaller than the coherence length, because the SHG scaling with the grain size becomes material specific.

Optical frequency conversion through phase match- ing in birefringent nonlinear (χ(2)) crystals has enabled a variety of applications in laser technology [1, 2] and plays a key role in quantum source schemes [3]. The birefringence provides an orientation- and polarization- dependent refractive index, which is used to compen- sate for the phase lag accumulated by the mixing waves. This avoids the destructive interference of the generated waves, which starts to occur at lengths larger than the co- herence length in any not phase-matched configuration. Random quasi-phase-matching (RQPM) is an alternative approach for removing destructive interference in optical frequency conversion [4, 5]. It relies on the disordered dis- tribution of the χ(2)-domains of certain media, such as polycrystalline materials [5–7], scattering powders [8–11] and bottom-up assembled photonic structures [12, 13]. Under a pump excitation the domains, or grains, gener- ate nonlinear waves with random phases and amplitudes. This leads to the cancellation of the interference terms and to the linear accumulation of the generated power with the number of domains. While RQPM is gener- ally less efficient than phase matching, it provides numer- ous advantages, such as an ultra-broad acceptance band- width (tunability of the pump over hundreds of nanome- ters), the use of low-cost materials, and relaxed con- straints on the polarization and the angle of incidence of the pump. These features make RQPM attractive for a variety of applications, such as optical-parametric- oscillators [14], ultrafast mid-infrared lasers [15], and ul- trafast autocorrelators [16]. The interest on RQPM has been largely focused on isotropic (i.e. non-birefringent) crystals such as ZnSe, both experimentally and theoret- ically [5, 17, 18]—one reason for this is that RQPM en- ables taking advantage of the large nonlinearity of these isotropic crystals, even if they are non-phase-matchable. First modeling of RQPM relied on the scalar approxima-

∗ [email protected]

tion of both the optical field and the χ(2)-susceptibiliy of the grains [17, 19]. Very recently, more comprehensive vectorial models have been developed to study the non- linear speckle statistics [18] and the supercontinuum gen- eration from isotropic disordered polycrystals [20]. SHG in birefringent disordered materials has only been mod- eled by averaging over the single grain generation, with- out considering the effects of the propagation through the birefringent medium on the polarization states [21, 22]. Up to now, no comprehensive model that explicitly ac- counts for the birefringence in RQPM has been presented.

Here, we introduce a vectorial model that considers the full three dimensional rotation (i.e. full χ(2)-tensor) as well as the birefringence of each grain. The generation and propagation of the waves is calculated from grain-to- grain, considering the phases of the ordinary and extraor- dinary beam components separately. This is done within the approximation of no scattering at the grain-to-grain boundaries. We explore the effects of the birefringence on RQPM by calculating the second-harmonic genera- tion (SHG) in disordered assemblies of lithium niobate (LiNbO3) and barium titanate (BaTiO3). We find that in general the birefringence is beneficial for RQPM. In monodispersed assemblies, the birefringence relaxes the grain size dependence of the SHG efficiency. In poly- dispersed assemblies, it introduces an efficiency enhance- ment of up to 54% compared to an isotropic reference material. Thanks to the birefringence, our model can simulate grains in a phase-matchable regime, in which the SHG enhancement increases linearly with the grain size. This allows us to draw a comparison to the powder- characterization technique of Kurtz and Perry [8, 22], which is widely applied to identify the phase-matchability of a crystalline material. Contrary to the established be- haviour at large grain sizes, we find that the SHG scal- ing with the grain size cannot unequivocally identify the phase-matchability of a crystal when the grain size is smaller than the coherence length.

ar X

iv :2

01 1.

10 42

9v 1

I. MODEL

The presented model considers a disordered three dimensional cuboid structure, consisting of quadratic (χ(2) 6= 0), birefringent, crystalline grains, as depicted in Fig. 1a. Similarly to other models [17, 18], the three di- mensional problem is reduced to a one dimensional prob- lem by breaking down the cuboid into multiple paral- lel one dimensional sticks. The SHG of each individual stick is calculated separately. Fig. 1b shows one disor- der configuration of such a stick, in which the grains have random sizes and orientations. The size Xn is ran- domly chosen from a Gaussian distribution with an av- erage grain size X and a polydispersity σ. The random orientation is defined through the rotation between the lab frame (a,b,c) and the crystal frame of each grain (x,y,z), with the Euler angles (, ϑ, γ)n, as shown in Fig. 1e. For this, the lab frame axes are defined as the c-axis parallel to the propagation direction k and the two orthogonal directions a and b, while the z axis is the optic axis of the crystal. For a uniform distri- bution of crystal orientations, we choose the rotation around z as ∈ [0, 2π], the angle between k and z as ϑ = arccos(u) with u ∈ [−1, 1] [18], and the rotation around k as γ ∈ [0, 2π]. The refractive indices of the ordinary (o) and extraordinary (e) axes are given by no

and ne(ϑ) = (

)−1/2 , with ne

the extraordinary refractive index at ϑ = π/2 [1]. A visu- alization of the calculation process in one single grain is shown in Fig. 1d. The incoming beam (pump) is defined as the plane wave (red)

E(ω) = (eaeiφa cosβ + ebeiφb sinβ)Eωe i(kc−ωt)

with amplitude Eω, frequency ω, wavevector k, the start- ing phases φa and φb, and a polarisation angle β in the lab frame. The vectors ea and eb are the unit vectors along the a and b axes. At the beginning of the grain, the elec- tric fields in the lab frame Elab, are transformed into the reference frame of the respective crystal Ecry = R ·Elab

(Fig. 1e), where R = Z1()X2(ϑ)Z3(γ) is the Euler- transformation matrix for a rotation around the original z-axis (Z1 = z) by , the new x-axis (X2 = o) by ϑ and final z-axis (Z3 = k) by γ (see Supplementaries II). In the crystal frame (Fig. 1d), the beams are decomposed into their components along the o and e axes and each polarisation combination of the pump (oo, eo, oe, ee) gen- erates a second-harmonic field Eugen(2ω,Xn) (blue) along

u ∈ {o, e}, which is given at the end of the nth single grain according to:

Eugen(2ω,Xn) = ∑

v,w

i(2ω)2

u 3Xn

(1) With the phase mismatch ku,vw = kv(ω) + kw(ω) − ku(2ω), the wave vector ku3 of the second-harmonic along u, and Pu,vw = eu,P vw the second-harmonic po- larization along v, w ∈ {o, e} projected onto the o/e-

FIG. 1. (a) Sketch of a three dimensional disordered assembly of second-order nonlinear grains, consisting of multiple par- allel one dimensional sticks. (b) Each stick contains grains of varying size Xn and orientation (, ϑ, γ)n, represented by the variation in colour. (c) Phasor (an) representation of the interference between the second-harmonic waves gener- ated by the grains within the stick. Each stick corresponds to a single random walk in the SHG complex plane, in which the step length is the amplitude of the second-harmonic field. (d) Schematics of the process to propagate, generate and in- terfere the beams. The input (left) is transformed into the crystal frame, propagated, summed with the generated SHG, and transformed back into the lab frame. (e) Depiction of the angles between the crystal frame (x,y,z) and the lab frame (a,b,c) with the transformation matrix R. β is the polarisa- tion angle of the input beam in case of a linearly polarized beam (φa = φb). The ordinary/extraordinary axes are indi- cated with o and e.

axis (eu unit vector along u ∈ {o, e}), where P vwi = 2ε0 ∑ jk dijkE

v jE

w k . The second-order nonlinear tensor

dijk is used in its contracted matrix form to calculate P vwi (see Supplementaries II). The pump E(ω, 0), as well as the total second-harmonic from all previous crystals Epre(2ω, 0) are propagated through the grain. For both beams, the components along the o and e axis are prop- agated separately: Eu(ω,Xn) = Eu(ω, 0)eik

u(ω)Xn . At the end of the grain, the second-harmonic from the pre-

3

vious grains is summed with the second-harmonic gener- ated in the current grain Eutot(2ω,Xn) = Eupre(2ω,Xn) + Eugen(2ω,Xn) (* in Fig. 1d). The amplitude, polarisation and phase of the fields is explicitly considered in every step. This way, the model can account for interference ef- fects. The fields of the propagated pump Eu(ω,Xn) and the total second-harmonic field Eutot(2ω,Xn) are trans- formed back into the lab frame, forming the output of the nth grain. To simulate the propagation of the light through the stick, we implemented a folding algo- rithm, which iteratively processes the sequence of grains. In each step, it takes the data of the current element (grain n) of the sequence and the result of the previous step (grain n−1) as input. The information is processed to generate the output of the nth grain which then forms the input of the (n+ 1)th grain. The SHG intensities of each stick Istick = cε0(|Eatot|2 + |Ebtot|2)/2 are averaged to yield the intensity of the cuboid. The model assumes an undepleted pump, no absorption within the grains, no reflections at the grain-to-grain interfaces, and the prop- agation only in the forward direction (no walk-off angle).

As an initial test of the algorithm, we computed the SHG from structures characterised by mono- and poly- dispersed grain sizes without randomisation of the grain orientation. The system behaves identical to a single crystal, periodically showing a totally constructive and destructive SHG along the length of the system. As ex- pected, there is no dependence on the size distribution of the grains (see Supplementaries III). When introduc- ing disorder in grain orientation and grain size, the SHG intensity of the single stick depends strongly on the spe- cific disorder configuration. In this case, the SHG in- terference along the stick corresponds to the trajectory of a single random walk in the complex plane, as de- picted in Fig. 1c. As such, the SHG intensity of a single stick cannot be correlated with the number of grains N . Only upon averaging the intensities of multiple sticks (i.e. along the transverse dimensions of the cuboid), the total SHG intensity grows linearly with N , providing evidence of RQPM [17]. To quantitatively study the influence of birefringence, we introduce the isotropic analogue of a birefringent material, defined as the material that has the same χ(2)-tensor as the original material, but with ne = no. Hence, the coherence length of the isotropic analogue Liso

c is not angle dependent. This stands in contrast to the coherence length in a birefringent mate- rial Lbir

c (, ϑ, γ)n, which depends on the angle, as well as the combination of beam polarizations. Thus, a random distribution of the grain orientations does not affect the coherence length of isotropic grains, while it randomises the coherence length of birefringent grains.

II. RESULTS

Monodispersed Assemblies.— One noteworthy result of this study, which is not exclusively related to birefrin- gence, is that even monodispersed structures (without

FIG. 2. Scaling of the SHG intensities with the number of grains N in birefringent LiNbO3 and in its isotropic analogue at a pump wavelength of 930 nm. SHG intensities are aver- aged over 1000 sticks, leading to a linear growth. Its slope represents the SHG efficiency for a certain grain size, and the shaded area shows the possible efficiencies in monodispersed assemblies. The insets explicitly show the SHG intensity in monodispersed assemblies only as a function of the grain size X for N = 100. In polydispersed assemblies (σ = 30%) with large grains (X > 3 Liso

c in the isotropic and X > 8 Liso c

in the birefringent material) the efficiency has a stable value corresponding to the dotted line. (a) The isotropic analogue has zero-efficiency minima when X is an even multiple of Liso

c , and efficiency maxima when X is an odd multiple of Liso

c . (b) The birefringent assembly has its minimum at X = 9.25 Liso

c

and its maximum at X = 3.47 Liso c .

size randomisation) sustain RQPM, as long as the grains are randomly oriented. This is shown in Fig. 2a-b for LiNbO3. The SHG efficiency per grain is measured by the slope of the linear growth, which depends on the grain size X. Its variation is represented by the shaded area and can be seen in the insets of Fig. 2a-b, which report the SHG intensity as a function of the grain size. The isotropic analogue, Fig. 2a, shows a maximal efficiency when X is an odd multiple of Liso

c and a minimal (zero) efficiency when X is an even multiple of Liso

c . The latter case corresponds to the totally destructive SHG inter- ference within the single grains. This is consistent with the results of Vidal. et al. [17] at low polydispersity. The effect of the birefringence is shown in Fig. 2b. The maximal as well as the minimal efficiency is increased compared to the isotropic analogue. In particular, the lower bound of the cone has a non-zero slope and the SHG never vanishes. Indeed, each birefringent grain has an orientation-dependent coherence length Lbir

c (, ϑ, γ)n, prompting that there is no specific grain size at which to- tal destructive interference occurs for all grains. BaTiO3

4

shows the same effect, but with a narrower cone of possi- ble efficiencies (see Supplementaries IV). The considered case of monodispersed assemblies highlights that polydis- persity is neither a sufficient nor a necessary condition to achieve RQPM. This stands in contrast to the random orientation of grains, which plays a key role in reaching the RQPM regime.

Polydispersed Assemblies.— In Fig. 3a the SHG in- tensity of LiNbO3 assemblies (red) and of their isotropic analogue (blue) is shown for an increasing average grain size 0 ≤ X ≤ 20 Liso

c , a polydispersity σ = 30%, and a fixed number of grains N = 100. Both curves follow the expected trend for RQPM [17]. In the small grain regime (X > Liso

c ) the SHG intensity grows with the grain size without an appreciable difference between the bire- fringent and the isotropic case. Maximal intensities are reached when X = Liso

c , for the isotropic analogue and for slightly larger grains in birefringent LiNbO3. After an initial peak, the SHG gets independent of the average grain size, at ≈ 3 Liso

c for the isotropic analogue and at ≈ 8 Liso

c for the birefringent LiNbO3. In this stabilised large-grain regime, the SHG intensity of the birefringent LiNbO3 is significantly larger than the stable value of the isotropic analogue. Specifically, we observe a peak enhancement of 54 ± 2% at 3 Liso

c . The effect is weaker in BaTiO3, where the birefringence leads to an SHG en- hancement of 9.25± 0.8% (see Supplementaries IV). The enhancement can also be seen on the slope of the of dot- ted lines in Fig. 2a-b, which report the linear scaling of the SHG intensity for assemblies with polydispersed grains at large grain sizes.

The origin of this overall enhancement lies in the dis- tribution of the SHG intensities generated by the indi- vidual grains Igen = cε0(|Eogen|2 + |Eegen|2)/2 within the cuboid, which are shown in Fig. 3b for both the bire- fringent (red) and the isotropic (blue) LiNbO3. These two SHG intensity distributions have been obtained by extracting Igen of the individual grains from the com- plete simulation depicted in Fig. 1d, thus considering the specific polarization state of the pump (phase retarda- tion between the o and e components) that the propaga- tion through the previous birefringent grains introduced. The birefringence significantly widens the range of pos- sible SHG intensities in the individual grains, due to the increased coherence lengths Lbir

c (, ϑ, γ)n > Liso c for cer-

tain grain orientations. Consequently, the average SHG intensity of the individual grains of birefringent LiNbO3

is 54.1± 0.3% higher than the isotropic analogue. Simi- larly for BaTiO3, the enhancement is 9.24± 0.1%, whose single-grain SHG intensity distribution is shown in the Supplementaries IV. The enhancements of Igen are con- sistent with the enhancement of the assembly calculated by considering the vectorial propagation of all compo- nents. We highlight that the birefringence is only bene- ficial in grains larger than the isotropic coherence length Xn > Liso

c . In smaller grains, the grain size Xn, rather than the coherence length, is the length scale limiting their SHG intensity (see Supplementaries V). To under-

FIG. 3. (a) Scaling of the SHG intensity with the average grain size for disordered assemblies of isotropic LiNbO3, bire- fringent LiNbO3, and birefringent LiNbO3 in the single grain (SG) approximation (single grain average ×N). The assem- blies have a grain size polydispersity σ = 30%, a fixed number of grains per stick N = 100, an averaging over 1000 sticks, and are simulated at a pump wavelength of 930 nm. At this wave- length, phase matching in LiNbO3 is not possible. (b) Proba- bility distributions of the SHG intensities generated by the in- dividual grains within the assembly (X = 3 Liso

c and σ = 30%) for isotropic LiNbO3, birefringent LiNbO3, and birefringent LiNbO3 in the single grain (SG) approximation (N = 1, lin- early polarized input beam). Probabilities are calculated as the relative frequency of appearance of an SHG intensity value over 107 grains. The SHG binning is 0.002. The SHG intensi- ties are multiplied by 100 to be directly comparable with the intensities of the 100-grain-assemblies in (a).

line the importance of modeling the phase propagation between the grains, we calculated the SHG scaling also in the single grain (SG) approximation, i.e. by consid- ering randomly oriented grains that are independently illuminated with a linearly polarized pump. Their aver- age SHG is then multiplied by N to get the SHG effi- ciency of the assembly ISG

tot = N × ISG gen. As shown in

Fig. 3a (grey line), the SG approximation overestimates the SHG enhancement in the birefringent assembly of LiNbO3 almost by a factor 2. This is because the SG approximation ignores the retardation…